Assembling Photoluminescent Silicon Nanocrystals into Periodic ... Assembling Photoluminescent...
Embed Size (px)
Transcript of Assembling Photoluminescent Silicon Nanocrystals into Periodic ... Assembling Photoluminescent...
Assembling Photoluminescent Silicon Nanocrystals into Periodic Mesoporous Organosilica Min Guan,†,‡ Wendong Wang,‡ Eric J. Henderson,‡ Ömer Dag,‡,§ Christian Kübel,∥,⊥
Venkata Sai Kiran Chakravadhanula,∥ Julia Rinck,# Igor L. Moudrakovski,∇ Jordan Thomson,‡
Jeffrey McDowell,‡ Annie K. Powell,∥,○ Haixia Zhang,*,† and Geoffrey A. Ozin*,‡
†Department of Chemistry, Lanzhou University, Lanzhou 730000, China ‡Materials Chemistry and Nanochemistry Research Group, Center for Inorganic and Polymeric Nanomaterials, Chemistry Department, University of Toronto, 80 St. George Street, Toronto, Ontario, Canada M5S 3H6 §Department of Chemistry, Bilkent University, 06800 Ankara, Turkey ∥Institute of Nanotechnology, Karlsruhe Institute of Technology (KIT), Hermann-von-Helmholtz-Platz 1, D-76344 Eggenstein-Leopoldshafen, Germany
⊥Karlsruhe Nano Micro Facility, Hermann-von-Helmholtz-Platz 1, D-76344 Eggenstein-Leopoldshafen, Germany #DFG Center for Functional Nanostructures (CFN), Karlsruhe Institute of Technology, Wolfgang-Gaede-Straße 1a, 76131 Karlsruhe, Germany ∇Steacie Institute for Molecular Sciences, National Research Council of Canada, Ottawa, Ontario, Canada K1A 0R6 ○Institute of Inorganic Chemistry, Karlsruhe Institute of Technology, Engesserstrasse 15, 76131 Karlsruhe, Germany
*S Supporting Information
ABSTRACT: A contemporary question in the intensely active field of periodic mesoporous organosilica (PMO) materials is how large a silsesquioxane precursor can be self-assembled under template direction into the pore walls of an ordered mesostructure. An answer to this question is beginning to emerge with the ability to synthesize dendrimer, buckyball, and polyhedral oligomeric silsesquioxane PMOs. In this paper, we further expand the library of large-scale silsesquioxane precursors by demonstrating that photoluminescent nanocrystalline silicon that has been surface-capped with oligo(triethoxysilylethylene), denoted as ncSi:(CH2CH2Si(OEt)3)nH, can be self-assembled into a photoluminescent nanocrystalline silicon periodic mesoporous organosilica (ncSi-PMO). A comprehensive multianalytical characterization of the structural and optical properties of ncSi-PMO demonstrates that the material gainfully combines the photoluminescent properties of nanocrystalline silicon with the porous structure of the PMO. This integration of two functional components makes ncSi-PMO a promising multifunctional material for optoelectronic and biomedical applications.
■ INTRODUCTION Since the first reports on the synthesis of periodically ordered mesoporous silica and aluminosilica through template-directed self-assembly,1−3 the concept of using a sacrificial template to direct the self-assembly has been extended to a rich compositional array of periodic mesoporous materials, which now includes metal oxides,4,5 metal chalcogenides,6,7 metal phosphates,8
metals and semimetals,9−14 carbon,15,16 and organosilica.17−21 In most syntheses, an amphiphilic template drives the separation of mesodomains and organizes small molecular precursors into ordered mesostructures. The ability of an amphiphilic template to organize and the ability of a precursor to diffuse put a practical limit on the size of the precursor for a successful coassembly. It is expected that large precursors are more difficult to assemble than small precursors. However, polymers,22 dendrimers,23 polyhedral oligomeric silsesquioxane,24 C60 molecules,
25 and nanoparticles26
have been incorporated into the mesoporous framework through template-directed self-assembly. Although they are mostly the
results of pure scientific curiosity, these synthetic feats have further extended the horizons of mesoporous materials and inspired the design of properties and functions for applying these materials in such areas as sensors, catalysis,27 nanoelec- tronics,28−30 light harvesting,31 energy storage and conservation,32
water purification,33 drug delivery,34 and biomedical imaging.35
The use of mesostructured materials in optical applications promises versatile processing strategies for fibers, spheres, films, and lithographic patterns with designed mechanical stability, wettability, and high loading of photoactive species.36,37 Early reports on the incorporation of photoactive species placed dye species in the hydrophobic regions of the micelle templates.36,37
Recent efforts focusing on the synthesis of luminescent forms of periodic mesoporous organosilica (PMO) have aimed at the inclusion of large conjugated structures in the pore walls31 in
Received: October 10, 2011 Published: April 18, 2012
© 2012 American Chemical Society 8439 dx.doi.org/10.1021/ja209532e | J. Am. Chem. Soc. 2012, 134, 8439−8446
order to preserve the pore space for further materials designs, such as the loading of another photoactive species to enable light harvesting.38 The chromophores in these luminescent PMOs are conjugated π structures. Compared with these organic chromophores, photoluminescent inorganic nanocryst- als have the advantage of high resistance against photobleaching and tunable size-dependent absorption and emission spectra.39
Nanocrystalline silicon (ncSi) is particularly attractive because of its expected biocompatibility, which makes it one of a growing class of “green” nanomaterials.40 The current methods of making photoluminescent ncSi-embedded mesoporous thin films and powders involve the growth of nc-Si in/on the pore walls by either chemical vapor deposition41 or metamorphic transformation of mesoporous hydridosilica (meso-HSO1.5) into mesoporous ncSi/SiO2, with the latter exhibiting stronger photoluminescence (PL).42 Incorporating ncSi into mesopo- rous materials may further hold promise in areas such as lighting, lasers, drug delivery, and bioimaging. Here we report the synthesis of photoluminescent nano-
crystalline silicon periodic mesoporous organosilica (ncSi-PMO) through template-directed self-assembly. The hydride-terminated surface of the ncSi was first capped with triethoxysilylethylene (TESE) oligomers through hydrosilylation with TESE. The capped ncSi was then coassembled with tetraethyl orthosilicate (TEOS) using Pluronic P123 under acidic conditions. We expect this new class of ncSi-PMO materials to show potential in optoelectronic and biomedical applications.
■ RESULTS AND DISCUSSION Freestanding silicon nanocrystals synthesized through high- temperature processing of hydridosilicate glass and subsequent HF etching of the ncSi−silica composite possess H-terminated surfaces.43 This H-terminated ncSi is hydrophobic and not soluble in water or ethanol, which are the usual solvents for syntheses of mesostructured materials. To enable self-assembly, the ncSi surface was first capped with oligo(TESE) through thermally initiated hydrosilylation (Figure 1). The oligo(TESE) layer makes the ncSi precursor soluble in ethanol (Figure 2a), and its ethoxysilane groups, after being hydrolyzed and polycondensed, provide bonding that stabilizes the porous gel network. The PL spectrum of the pure ncSi:(CH2CH2Si- (OEt)3)nH dissolved in ethanol (Figure 2b) displays a peak at 615 nm upon excitation at 330 nm. The chemical structure of ncSi:(CH2CH2Si(OEt)3)nH was
analyzed by FT-IR spectroscopy, UV−vis spectroscopy, liquid- phase NMR spectroscopy, and gel-permeation chromatography (GPC) (Figure 3). The IR spectrum of ncSi:(CH2CH2Si- (OEt)3)nH (Figure 3a) shows characteristic C−H vibrations at around 2900 and 1390 cm−1, Si−O−C vibrations at around 1100 cm−1, very weak Si−H vibrations at around 2100 cm−1,
and, as anticipated, little evidence for CC vibrations at 1600−1700 cm−1, suggesting almost complete reaction of the surface hydride groups on the ncSi and of the monomeric TESE. The UV−vis absorption spectrum of pure ncSi: (CH2CH2Si(OEt)3)nH (Figure 3b) has a broad absorption in the 200−500 nm region, predominantly originating from the ncSi core. The 1H NMR spectrum in CDCl3 (Figure 3c) shows resonances due to the ethoxy groups at 3.79 and 1.20 ppm and resonances due to the oligomer backbone at 0.56 and 1.48 ppm, the latter overlapping with a broad resonance attributed to water (1.59 ppm). The samples contained less than 2% unreacted TESE, as calculated by integrating the vinyl
Figure 1. Scheme for the synthesis of nanocrystalline silicon surface-capped with oligo(TESE), denoted as ncSi:(CH2CH2Si(OEt)3)nH, achieved through thermally initiated hydrosilylation of ncSi:H.
Figure 2. (a) Photos of ncSi:(CH2CH2Si(OEt)3)nH in ethanol solution displaying photoluminescence under UV light and (b) the corresponding PL spectrum with a peak at 615 nm.
Journal of the American Chemical Society Article
dx.doi.org/10.1021/ja209532e | J. Am. Chem. Soc. 2012, 134, 8439−84468440
protons (5.6−5.9 ppm). The spectrum appears virtually identical to that of pure oligo(TESE). The additional peak in the high-molecular-weight region (log Mw ≈ 4.5) in the chromatogram of ncSi:(CH2CH2Si(OEt)3)nH (Figure 3d), in comparison with that of pure oligo(TESE), indicates successful grafting of the oligomer onto the surface of ncSi. The precursor ncSi:(CH2CH2Si(OEt)3)nH was further
analyzed using high-resolution transmission electron micros- copy (HRTEM) and energy-filtered TEM (EFTEM).44
EFTEM collects only electrons that have lost a specific amount of energy as a result of the electron−specimen interaction and is advantageous over the other techniques for characterization of Si nanoclusters and nanoparticles.45 It generates a chemical map of the species of interest with a very high spatial resolu- tion.